β Sheets Not Required: Combined Experimental and Computational ...
Embed Size (px)
Transcript of β Sheets Not Required: Combined Experimental and Computational ...
Sheets Not Required: Combined Experimental and ComputationalStudies of Self-Assembly and Gelation of the Ester-ContainingAnalogue of an Fmoc-Dipeptide HydrogelatorKevin M. Eckes, Xiaojia Mu, Marissa A. Ruehle, Pengyu Ren, and Laura J. Suggs*
Department of Biomedical Engineering, The University of Texas at Austin, 107 W. Dean Keeton St. Stop C0800, Austin, Texas78712, United States
*S Supporting Information
ABSTRACT: In our work toward developing ester-containing self-assembling peptides as soft biomaterials, we have found that afluorenylmethoxycarbonyl (Fmoc)-conjugated alanine-lactic acid (Ala-Lac) sequence self-assembles into nanostructures that gelin water. This process occurs despite Fmoc-Ala-Lacs inability to interact with other Fmoc-Ala-Lac molecules via -sheet-likeamideamide hydrogen bonding, a condition previously thought to be crucial to the self-assembly of Fmoc-conjugated peptides.Experimental comparisons of Fmoc-Ala-Lac to its self-assembling peptide sequence analogue Fmoc-Ala-Ala using a variety ofmicroscopic, spectroscopic, and bulk characterization techniques demonstrate distinct features of the two systems and show thatwhile angstrom-scale self-assembled structures are similar, their nanometer-scale size and morphological properties diverge andgive rise to different bulk mechanical properties. Molecular dynamics simulations were performed to gain more insight into thedifferences between the two systems. An analysis of the hydrogen-bonding and solvent-surface interface properties of thesimulated fibrils revealed that Fmoc-Ala-Lac fibrils are stronger and less hydrophilic than Fmoc-Ala-Ala fibrils. We propose thatthis difference in fibril amphiphilicity gives rise to differences in the higher-order assembly of fibrils into nanostructures seen inTEM. Importantly, we confirm experimentally that -sheet-type hydrogen bonding is not crucial to the self-assembly of short,conjugated peptides, and we demonstrate computationally that the amide bond in such systems may act mainly to mediate thesolvation of the self-assembled single fibrils and therefore regulate a more extensive higher-order aggregation of fibrils. This workprovides a basic understanding for future research in designing highly degradable self-assembling materials with peptide-likebioactivity for biomedical applications.
INTRODUCTIONPeptide-based low-molecular-weight gelators (LMWG) holdgreat promise for use as biomaterials for tissue engineering.These short peptides, typically conjugated to an N-terminalhydrophobic protecting group, can be triggered to self-assembleinto gel-forming nanofibrillar structures via a pH change,solvent switch, and/or heating and subsequent cooling.1
Because of this ability to trigger their self-assembly, peptide-conjugate LMWGs may be ideal for placement by injection;many polymer gel systems previously proposed for use asbiomaterials require photoinitiators for cross-linking by UVlight, which is highly scattered by biological tissues. Peptidesalso have inherent sequence-specific biological activity, whichmay be easily leveraged to enhance therapeutic cell signaling or
promote cellbiomaterial adhesion. Finally, with recentexamples of these peptide-based LMWGs using naturallyoccurring hydrophobic N-protecting groups (such as DNAbases2) or groups with known biocompatibility (such asibuprofen3 and naproxen4) these materials are likely to behighly biocompatible and possibly even actively antibacterialand anti-inflammatory.While peptide-based gels possess many properties favorable
for use as biomaterials, they are not readily degradable bynonenzymatic means at physiological pH and temperature. For
Received: February 20, 2014Revised: March 31, 2014Published: April 22, 2014
2014 American Chemical Society 5287 dx.doi.org/10.1021/la500679b | Langmuir 2014, 30, 52875296
This is an open access article published under an ACS AuthorChoice License, which permitscopying and redistribution of the article or any adaptations for non-commercial purposes.
this reason, our group has been developing synthetic protocolsfor ester-containing depsipeptides that have side-chainfunctionality analogous to that of peptides. As esters have ahalf-life over 1000 times shorter than that of amide bonds,5
depsipeptides are prone to hydrolysis over a time scale relevantto wound healing and tissue remodeling processes. We havedeveloped didepsipeptide units (containing a single N-protected amino acid conjugated to an -hydroxy acid via anester linkage) that can be coupled to other amino acids ordepsipeptide units using standard solid-phase peptide synthesischemistries.6
The general structure of a depsipeptide unit is almostidentical to that of a fluorenylmethyloxycarbonyl (Fmoc)-protected dipeptide. Several Fmoc-dipeptides have beenreported to self-assemble into nanofibrillar structures to formhydrogels, and it has been hypothesized that -sheet-likehydrogen bonding between amide bonds on adjacent moleculeshelps to drive self-assembly and stabilize the supramolecularnanostructures.1,7 We recently developed computationalsimulation techniques to model the self-assembly of Fmoc-Ala-Ala (i.e., Fmoc-AA), a simple Fmoc-dipeptide with uniformside-chain functionality, and we found that amideamidehydrogen bonding comprises less than 10% of the total numberof hydrogen bonds between Fmoc-Ala-Ala molecules in asupramolecular assembly.8 Given these results, we hypothesizedthat Fmoc-depsipeptides may be able to self-assemble into gel-forming nanostructures under conditions similar to those for ananalogous Fmoc-dipeptide.A depsipeptide analogue of an Fmoc-dipeptide contains an
ester bond in place of an amide bond. Because esters lack ahydrogen bond donor, they are unable to interact with adjacentester bonds via hydrogen bonding. Therefore, a depsipeptideanalogue serves as an ideal model for testing whether -sheet-like amideamide hydrogen bonding is truly a requirement forthe self-assembly and gelation of N-terminal hydrophobicprotected peptides. In this article we show that Fmoc-Ala-Lac(i.e., Fmoc-ALac), the depsipeptide analogue of the knownLMWG Fmoc-Ala-Ala, indeed undergoes self-assembly andgelation despite its inability to form specific -sheet-likehydrogen bonds. Morphological characterization of the gelsshows striking similarities, whereas spectroscopic and mechan-ical analyses reveal distinct differences in the two systems thatare attributable only to differences in the extent of hydrogenbonding. We also performed computational simulations of theself-assembly process of these molecules to compare thefeatures of Fmoc-Ala-Lac Fmoc-Ala-Ala that are not readilymeasurable by experimental means, including the number andnature of hydrogen bonds formed, the intrafibril stability, andthe fibrilfibril aggregation potential. When combined, theresults of the experimental and computational work hereinprovide critical information needed for the successful design ofnew degradable, injectable, and biologically active biomaterialsbased on modified peptides.
EXPERIMENTAL SECTIONFmoc-L-Ala-L-Ala-OH. The N-protected dipeptide was purchased
from Bachem, Inc. (Torrance, CA) and used without furtherpurification.Fmoc-L-Ala-L-LacOH Synthesis. Fmoc-L-Ala-L-LacOH was
synthesized using the general strategy for depsipeptide unit synthesisintroduced by Nguyen et al.6 Synthesis and purification details as wellas identification and purity analysis though NMR and HPLC-MS canbe found in the Supporting Information.
Gel Preparation. All gels characterized in this study were preparedusing a pH switch method. To a solution of either Fmoc-AA or Fmoc-ALac, 1 equiv of 0.5 M NaOH was added in order to deprotonate anddissolve the molecules. This mixture was vortex mixed and sonicatedjust until clear and then immediately added to a small volume of 1equiv of 0.1 M HCl in a separate vial to reduce the gel inhomogeneity.Gelator solutions at high pH were always prepared fresh and gelledimmediately to prevent Fmoc removal. Although related work wouldindicate that ester-containing Fmoc-ALac gels are relatively stable tohydrolysis over the time course of analysis experiments,9 to minimizethese effects only freshly prepared gels were analyzed. For 5 mg/mLgels, the final pH of Fmoc-AA gels was between 3.1 and 3.5, and thefinal pH of Fmoc-ALac gels was between 3.2 and 3.4.
Transmission Electron Microscopy (TEM). TEM samples wereprepared using 5 mg/mL gels. Approximately 10 L of gel was placedon the shiny side of a non-glow-discharged 300-mesh carbon-coatedcopper grid (Electron Microscopy Sciences, Hatfield, PA) and allowedto adsorb for 2 min. Excess gel and water were wicked away using filterpaper, and the grid was placed shiny side down on top of a 10 L dropof DI water for 30 s to wash away any salts. After wicking the washingwater with filter paper, grids were placed shiny side down on top of a10 L drop of 4% uranyl acetate in water for 1 min. Finally, the uranylacetate solution was wicked away using filter paper, and the grids wereallowed to dry completely before imaging. Samples were imaged onthe nanometer scale using a FEI Tecnai instrument with anacceleration voltage of 80 kV, and the AMT Advantage HR 1kX1kdigital camera associated with the instrument was used to producedigital micrographs.
Wide-Angle X-ray Scattering (WAXS). All gel samples wereprepared at 5 mg/mL as described above, allowed to dry slowly onsingle-crystal quartz slides over 48 h in a humid environment, and thendried completely in vacuo. Dried gel films were subjected to X-raysoperating at a wavelength of 1.54059 (Cu K1) on a Scintag X1 powder diffractometer. Diffraction patterns were analyzed usingJade v9.1.1 (Materi